Keywords: Paracetamol; Adsorption; Activated carbon; Chemical activation. Abbreviations: .... thiosulphate solution using starch as indicator. Surface area.
Available online www.jocpr.com
Journal of Chemical and Pharmaceutical Research, 2017, 9(3):56-68 Research Article
ISSN : 0975-7384 CODEN(USA) : JCPRC5
Removal of Paracetamol from Aqueous Solution by Adsorption onto Activated Carbon Prepared from Rice Husk Ndifor-Angwafor George Nche1*, Aurelien Bopda1, Donald Raoul Tchuifon Tchuifon1, Christian Sadeu Ngakou1, Idris-Hermann Tiotsop Kuete1 and Anagho Solomon Gabche1,2 1
Laboratory of Noxious Chemistry and Environmental Engineering, Department of Chemistry, University of Dschang, Dschang, Cameroon 2 Department of Chemistry, Faculty of Science, The University of Bamenda, Bambili, Cameroon _____________________________________________________________________________
ABSTRACT Removal of paracetamol from aqueous solution onto two activated carbons CANa1 and CANa2 obtained by the chemical activation of rice husk with sodium hydroxide was study in this work. The characterization of the activated carbons showed that the ph at zero charge was 6.80 for CANa1 and 6.54 for CANa2, while the pH of CANa1 was 7.10 and that of CANa2 was 7.13. from the adsorption of acetic acid, the specific surface areas were obtained as 178.13 m2/g for CANa1 and 104.82 m2/g for CANa2. The determination of the iodine number gave values 528.39 mg/g and 494.67 mg/g for CANa1 and CANa2 respectively. The kinetics of the adsorption was adequately described by the pseudo-second order and intraparticulate diffusion models. Concerning the equilibrium studies, the model of langmuir described best the adsorption on CANa1 while the model of freundlich described best the adsorption on CANa2. From the results obtained, CANa1 and CANa2 constitute effective adsorbents for the elimination of paracetamol from industrial waste water, the equilibrium is in according with the langmuir model, while the quantities adsorbed were 20.964 mg/g and 14.881 mg/g respectively. Keywords: Paracetamol; Adsorption; Activated carbon; Chemical activation Abbreviations: CANA1: activated carbon obtained by chemical activated of rice husk with NaOH as activating agent at 500°C; CANa2: activated carbon obtained by chemical activated of rice husk with NaOH as activating agent at 450°C _____________________________________________________________________________ INTRODUCTION The lack of appropriate treatment systems for effluents from pharmaceutical industries is responsible for introducing significant amounts of medicines into diverse aquatic ecosystems, thus creating serious environmental problems throughout the world. The production of pharmaceuticals has increased rapidly in the last decades, providing better health quality for humans and animals . The presence of these pharmaceuticals in the environment in concentrations in the µg/L or ng/L range poses the threat to aquatic organisms in terms of mutagenicity as well as currently unknown effects to humans. Pharmaceuticals originally from humans and feedstock wastewaters often found their way into surface water sources . Among the drugs frequently used in the world; analgesics and antiinflammatories are the most common, and they are widely consumed with or without medical prescription. Of these drugs, paracetamol stands out as being highly toxic to the liver, and it has a high potential for developing hepatitis . Paracetamol; an antipyretic/analgesic drug has been widely investigated because of its common use and because 56
NAG Nche et al J. Chem. Pharm. Res., 2017, 9(3): 56-68 __________________________________________________________________________________________ of the fact an overdose of it results in health problems such as acute hepatic failure, liver damage [4,5,6,7] and even death. To prevent the release of pharmaceuticals from industries into natural water sources, a number of conventional methods for the removal of organic pollutants are being investigated. These methods may be divided into three main categories: physical, chemical and biological. Often, in drug poisoning, the amount of drugs in the order of magnitude of many grams may have been ingested. This amount is close to the adsorption capacity of the activated carbons often used. As standard treatment, a dose of 50 g activated carbon has been shown to be effective as a gastro-intestinal decontaminant in human volunteers who ingested multiple drugs, although these investigations involved only sub-toxic drug [8-11]. Adsorption, one of the physical methods is generally considered to be an effective method for quickly lowering the concentrations of organic molecules in an effluent . The activated carbons have been previously used to remove lead from aqueous effluents. The most important commercial adsorbent is a carbonaceous material with a large surface area, high porosity, adequate pore size distribution and high mechanical strength . Activated carbons can be produced from different carbonaceous materials such as coal, wood, peat and agricultural wastes especially lignocellulosic by-products like pinewood , date’s stone , cola nut shells , and maize stalks . Recent progress of industrial technologies provides new application fields for activated carbons in super-capacitors, and the carbons are required to have the desired pore structure . The production of activated carbon from agricultural by-products has potential economic and environmental benefits. It converts unwanted, low value agricultural waste to useful, high value adsorbents. Activated carbons are increasingly being used to remove organic compounds and heavy metals of environmental and/ or economic concern  from waste streams. The aim of this study was to use rice husk; a local agricultural waste, to produce activated carbons, and to investigate the removal of paracetamol from aqueous solution using these activated carbons. MATERIALS AND METHODS Preparation of activated carbon The rice husk used in this work was collected from Ndop subdivision in the North-West Region of Cameroon. The rice husk was washed with tap water, then rinsed with distilled water to eliminate impurities and then dried under sunlight for 72 hours before activation. The ratio of impregnation is defined as the ratio of the mass of the activating agent to the mass of the dry biomass precursor. To produce an activated carbon with an impregnation ratio of 35%, 200 g of dried rice husk was put in contact with 350 mL of a 1.0 molar solution of NaOH. The mixture was kept for 30 minutes for activation to take place before being dried in an oven set at 105°C for 24 hours. The samples of impregnated rice husk were carbonized for 1 hour at 450°C and 500°C, at a heating rate of 5°C/min. The activated carbons obtained were labeled CANa1 for rice husk carbonized at 500°C and CANa2 for rice husk carbonized at 450°C. The carbonization was carried out in an electric furnace of mark ISUNU, which has an automatic regulation, and a temperature programmer coupled to it. The various activated carbons thus obtained were dried for 24 hours at the temperature of 105°C, before being crushed and filtered to obtain activated carbon of particles of sizes lower than 100 µm. Characterization of adsorbents Bulk density: A 15 cm3 specific gravity bottle was weighed empty, and later when carefully filled to the mark with powder activated carbon. The difference in the masses gave the mass of the powder activated carbon. The bulk density was calculated from the equation: (1) Moisture content A previously weighed crucible was weighed with 1 g of powdered air dried activated carbon. It was then placed on a hot plate maintained at 110 °C. After one hour, it was taken out and cooled in a desiccator before being weighed again. The ratio of the mass of the powder lost to its original mass gave the moisture content of the sample. Iodine number To gain further knowledge of the porous structure of activated carbon, the adsorption of iodine from liquid phase was adopted by other researchers in the characterization of sludge-based activated carbons [19,20]. The adsorption of aqueous I2 is considered a simple and quick test for evaluating the microporosity of activated carbons associated with pore diameter less than 2 nm. The iodine number, defined as the amount of iodine adsorbed per gram of 57
NAG Nche et al J. Chem. Pharm. Res., 2017, 9(3): 56-68 __________________________________________________________________________________________ activated carbon at an equilibrium concentration of 0.02 N, was measured according to the procedure established by the American Society for Testing and Materials . Activated carbon of mass 0.1 g, was mixed with 30 mL of 0.02 N iodine solutions and stirred for 3 hours. After filtration, 10 mL of the filtrate was titrated against 0.005 N sodium thiosulphate solution using starch as indicator. Surface area Another method of determining the specific surface area of adsorbent is based on adsorption of molecules of acetic acid , whose molecular surface area of 21 Å2 is close to that of nitrogen, N2 (16.2 Å2). To determine the specific surface area of the adsorbent, 20 ml of acetic acid solution of concentration ranging between 4x10 -3 and 8x10-3 M was put in contact with 0.1 g of activated carbon. This mixture was filtered after agitating for 60 minutes. The residual concentration of the acid was determined by the volumetric assay technique . The specific surface area SL (in m2/g) was determined using the equation (2): (2) Where N = 6.02x1023 mol-1 (Avogadro constant), SA = 21 Å2 (molecular surface area of acetic acid) and Qm maximum quantity of acid adsorbed as obtained from the isotherm of Langmuir. Batch adsorption Adsorption experiments were carried out by mechanical agitation at room temperature. For each run, 20 mL of paracetamol solution of known initial concentration (between 70-120 mg/L) was treated with a known weight of different activated carbon. After agitation, the solution was filtered, and the filtrate analyzed to obtain the residual of concentration paracetamol by using the UV/Vis spectrophotometer (Jenway, model 6715). Similar measurements were carried out by varying adsorbent doses, pH of the solution, ionic strength and the initial concentrations of the solution. The percentage removal (%R) of paracetamol, and the amount (Qe) of paracetamol adsorbed were calculated using the following expressions: (3) (4) C0 is the initial concentration of the phenol, Ce is its equilibrium concentration, Ct is the concentration of the paracetamol solution at the time t, V is the volume of the solution, and m is the mass of the absorbent. Effect of contact time To determine the effect of agitation time on the adsorption process, 0.1 g of ground adsorbent was agitated in a 20 mL solution of paracetamol of initial concentration 100 mg/L for different time intervals. At each time t, the solution was rapidly filtered and the residual concentration determined by spectrophotometer. The amount (Qe) of paracetamol adsorbed was calculated by using equation (4). Effect of amount of adsorbent In this set of experiments, different masses of the adsorbents ranging between 0.025 to 0.45 g were treated with 20 mL solution of the paracetamol of initial concentration 100 mg/L. Effect of initial pH For each adsorbent, the optimal mass of adsorbent obtained at the end of the preceding study was treated with 20 mL of aqueous solution of 100 mg/L of paracetamol in the pH range of 2.0 – 3.5. The adjustment was done by adding either HCl or NaOH. Kinetics of adsorption studies The kinetics experiments were conducted using a series of 20 mL solutions containing known amounts of adsorbent and concentrations of paracetamol. The solutions were vigorously agitated for increasing time intervals. At the end of each interval, the solution was analyzed in order to determine the residual concentration of paracetamol. A number of kinetic models were used to test the fit of the experimental data. These are: The pseudo-first order model The pseudo-first order equation is generally expressed as [22,23]: 58
NAG Nche et al J. Chem. Pharm. Res., 2017, 9(3): 56-68 __________________________________________________________________________________________ (5) Where and are the adsorption capacities at equilibrium and at time t, respectively (in mg/g) and K 1 is the rate constant for the pseudo-first order adsorption (1/min). After integration and applying boundary conditions that at t = 0, Qt= 0; and at t = t, Qt = Qt, the integrated form of equation (5) becomes: (6) The pseudo-second order model The pseudo-second order chemisorption kinetic equation [24,25] is expressed as Equation 7: (7) Where is the rate constant for the pseudo-second order adsorption (g/mg.min). For boundary conditions are that, at t = 0, Qt= 0; and at t = t, Qt = Qt, the integrated and rearranged form of equation (7) is: (8) In the equation (8),
is the initial rate for the adsorption
Intraparticle diffusion model The intra-particle diffusion model or the Weber and Morris equation  models the type of diffusion mechanism involved in adsorption processes. It is given here by equation (9): (9) Where is the intra-particle diffusion constant (mg/g.min). The linear form of this equation takes the following form . (10) Where; P is the percentage of paracetamol removed at instant t and a is a constant that depends on the adsorption mechanism. When intra-particle diffusion plays a significant role in controlling the kinetics of the sorption process, the plots of yield straight lines passing through the origin and the slope gives the rate constant, . However, when the transport of the solute molecules from the liquid phase up to the solid phase boundary plays the most significant role in adsorption, the liquid film diffusion model may be applied. Batch equilibrium experiments For each run, the adsorbent was mixed with 20 mL solution of paracetamol at different initial concentrations from 50-110 mg/L. The suspension was stirred for 60 minutes with different activated carbon. The amount of paracetamol adsorbed at equilibrium, Qe (mg/g) was calculated using equation (4). Equilibrium data were then fitted by using the isotherms of Langmuir, Freundlich, Dubinin-Radushkevich and Temkin. The Langmuir isotherm: The Langmuir adsorption isotherm is often used of the equilibrium of the adsorption of solutes from solutions. It is expressed as : (11) Where, Qe is the adsorption capacity at the equilibrium solute concentration, (in mg of adsorbate per g of adsorbent); Ce is the equilibrium concentration of adsorbate in solution (mg/L), while Q m is the maximum adsorption capacity corresponding to complete monolayer coverage expressed in mg of solute adsorbed per g of adsorbent. is the Langmuir constant in L of adsorbate per mg of adsorbent, and it is related to the energy of adsorption. Equation (11) can be rearranged in the linear form: (12) The factor of separation of Langmuir, RL, which is an essential factor characteristic of this isotherm is calculated by using the relation :
NAG Nche et al J. Chem. Pharm. Res., 2017, 9(3): 56-68 __________________________________________________________________________________________ (13) Where C0 is the higher initial concentration of paracetamol, while and Qm are the Langmuir constant and the maximum adsorption capacity respectively. The parameters indicate the shape of the isotherm as follows: RL values indicate the type of isotherm. when RL = 1 adsorption is linear; when 0 < RL< 1, it is favourable, when RL = 0, it is irreversible, while to be unfavorable, while when RL> 1, it is unfavorable. The Freundlich isotherm: The Freundlich isotherm is based on adsorption on a heterogeneous surface, and it is expressed as . (14) Where and linear form:
are empirical constants. By taking logarithms on both sides, the equation gives the more convenient
(15) A linear graph of ln Qe versus ln Ce gives the values of 1/n and ln Kf. The values indicate the type of isotherm as follows: to be irreversible while to be unfavorable > 1.
= 0; to be favorable 0